2 1-Porosity:a)Too rapid rise of temperature in the initial stage of curingb)Thick denture bases heated too rapidly.c)Lack of dough in the mold at the time of final closure.d)Lack of adequate pressure during polymerization.e)Packing the resin in a sticky rather than doughy stage.
4 2-Tooth movementsa) The use of plaster instead of stone in investing the trial denture .b) Incomplete closure of the flask .c) Excessive and rapid pressure during trial closure .d) Over packing of the mold with resin material before final closure ..
5 3 . Denture base and teeth breakage during Deflasking a) Careless flasking( knife blade hit teeth when removing stone cap) .b) Hammer used to tap denture out of the flask .
6 4 . Fractured or cracked teeth : causes :a) Improper Deflasking( use hammer)b) Packing the dough in the rubbery stage the material too stiff .c) Excessive and rapid application of pressure during trial packing .d) Setting the teeth directly on the stone cast .
7 5 . Crazing of acrylic resin base or acrylic teeth : crazing of resin consists of the formation of small cracks which may vary in size from microscopic dimension to the visible size it indicates beginning of fracture . cross linking of resin reduces this fault considerably .causes ;a) Stresses induced by the contraction of the resin around the tooth by rapid cooling .b) he use of solvents to remove wax from the mold before packing .C) Application of separating medium just before packing
8 6 . Bleaching of acrylic resin causes :a) Contamination of the acrylic resin with some acrylic solvents .b) under cured acrylic resin due to incorrect time and temperature of curing .c) incorporation of the tin foil substitute with the acrylic resin .d) incorporation of the jelly like material of wet cellophane into the resin .
9 7 . color streaks in the resin material: causes:a) improper mixing of the monomer and polymer .b) contamination of the resin mix with dirty hands or instrument .c) adding resin material in layers during trial packing .
10 8 . Sandy appearance of the resin material : Causes ;a) Too much delay in curing after packing [ more than 1\2 hour ] .b) Evaporation of the monomer liquid.c) Insufficient monomer in the mix (packing of a dry mix) .
11 9 . Stone adhere to the surface of the denture: Causes ;a) Insufficient separating medium on the mold before packing .b) The application of separating medium contaminated with stone .c) Incomplete elimination of wax during washing out thus rendering separating medium ineffective .
12 10 . Space between the teeth and resin base: Causes :a) Delayed curing leaving the flask without curing for a long time .b) The application of separating medium on the teeth